scientia research provide a cheap alternative to portland cement with properties that are acceptable
Post on 08-Sep-2019
Embed Size (px)
www.scientiaresearchlibrary.com tAvailable online a
Scientia Research Library ISSN 2348-0424 USA CODEN: JETRB4
Journal of Engineering And Technology Research, 2014, 2 (4):41-51
Durability of high –belite sulfate resisting cement pastes in MgSO4 solution H. El-Didamony[1a], A. Radwan[1b], I. Khattab, E.A. El-Alfi , Mona S. Mohammed
[1a]Faculty of Science, Zagazig University, EgyptNational Research Centre, Dokki, Cairo, Egypt
The influence of 4% MgSO4 solution on the durability of the sulfate resisting cement (SRC) pastes with different ratios of belite up to 9 months was studied. The relative resistance of hardened cement pastes against the aggressive solution was assessed by determining the compressive strength, free lime, bulk density, apparent porosity, total sulphate and the hydration products with the aid of TGA, XRD, SEM and IR spectroscopy. It was found that the chemically combined water, free lime and total sulphate contents decrease with increasing belite content. The SEM shows that, SRC pastes with higher ratio of belite showed good resistance in aggressive media compared to other cements.
Keywords: Sulfate resistance cement, Belite, Alite, Durability .
The Portland cement industry consumes large amounts of energy and produces huge quantities of CO2
. So, the authers made industrial trials for the production of belite cements at lower temperatures and lime saturation factors than for OPC. It was found that, the energy consumed during the production of the belite cement clinkers was less than that of OPC. Compared with the production of OPC less limestone was consumed and less CO2 evolved. Such low energy cements provide a cheap alternative to Portland cement with properties that are acceptable for many applications and the additional benefit of possible improved durability .1
The belite cement has the advantages in comparison with Portland cement as follows:
. It requires less water demand for normal consistency, and possesses higher mortar flow ability, more compatible with concrete admixture, and therefore offers better workability to concrete,
. Its strength increase more rapidly at later ages in spite of its much lower early strength . The strength of high belite cement at 90 and 180 days is higher than those of OPC at the same ages,
. It has lower heat of hydration and adiabatic temperature rise, less drying shrinkage and better resistance to chemical corrosion and to abrasion, which implies that it offers durability better than OPC.
1 1 Corresponding Author E-mail: Radwan_@hotmail.com
H. El-Didamony et al J. of Eng. & Techn. Res., 2014, 2(4):41:51
The resistant to sulphate attack of Portland cement with similar fineness and different chemical composition was investigated . It was observed that, under the SEM the cement with higher C3S content gypsum led to form in large veins parallel to the surfaces exposed to solution. However, in the low C3S cement gypsum was located throughout the sample. Ettringite was found in all cements. The authors concluded that lowering the C3S and C3A contents of cement improves its resistant to sulphate attack. Cement with low C3S (39%) and low C3A content (4.6%) had the best performance in sulphate environments. It exhibited the lowest strength drop and expansion.
The manufacture of high strength SRC was studied . It was found that the sulphate resistant character of cement is obtained by suitably adjusting the component of minerals in the clinker, lowering the C3S and C3A contents, promoting the C2S content and decreasing the gypsum addition improved physical-chemical properties of the cement.
Mixtuers of SRCs, (with 40 % and 74 % C3S content) and blended cements containing natural pozzolana or limestone filler were investigated . Expansions, flexural and compressive strength of mortar immersed until 1 year in sodium sulphate solution were measured. The sulphate resistance of Portland cement with high C3S content is very poor compared with low C3S cement. Addition of natural pozzolana provides the maximum sulphate resistant while the addition of 20% limestone filler declining sulphate resistant of low C3A cements. This behavior can be attributed to the reaction between SO4
and CH in the paste.
The aim of the present work is to study the durability of the prepared sulphate resisting cements having different belite contents in 4 % MgOS4 solution. The kinetics of hydration and mechanical properties of cement paste were determined. The hydration products were also identified by using SEM, XRD, TGA, and IR techniques.
MATERIALS AND METHODS
The materials used in this investigation were sulphate resistant Portland cement (SRC) provided from El-Masria Cement Company and belite prepared from pure chemicals. The chemical compositions of starting material are shown in Table (1).
Belite (β-C2S) was synthesized from reagent grade CaCO3 and pure ground sand (more than 99.5 % SiO2) in the proper molar ratio. The dry constituents of limestone and silica were mechanically mixed for 1/2 hour in a porcelain ball mill using two balls to attain complete homogeneity, then fired twice at 14500C for two hours soaking time using B2O3 (0.5%) as stabilizer to complete formation of belite phase. The belite phase was ground and kept in airtight container. The dry constituents of SRC and belite phase were mechanically mixed for 30 minutes in a porcelain ball mill to attain complete homogeneity. The samples were kept in airtight containers. Two cements B & C were prepared by mixing different amounts of belite with SRC. The phase composition of the prepared cements is shown in Table (2).
The mixing of the paste was done as described in a previous work . The pastes were moulded in 0.5 inch cubic moulds, cured in humidity chamber at 23+1 ºC for 24 hours, then demoulded and immersed in tap water up to 28 days (zero time). The samples were immersed in 4% magnesium sulfate solution as aggressive medium for 1, 3, 6, and 9 months. Three cubes representing each mix were tested for the compressive strength, free lime (7), apparent porosity and total sulfate. The hydration products of immersed sample were identified with the aid of TGA, XRD, SEM and IR spectroscopy.
H. El-Didamony et al J. of Eng. & Techn. Res., 2014, 2(4):41:51
RESULT AND DISCUSSION
The determined values of chemically combined water of the hardened cement pastes are graphically represented as a function of curing time in Figure (1). The combined water content increases with time and alite content for all cement pastes due to the increase of the hydration products. This is due to the higher activity of alite than belite. MgSO4 reacts with either C3AH6, C3(AF)H6 and the librated lime from the hydration of alite as wall as belite. The alite phase librates 3 moles of Ca(OH)2 in comparison to one mole of belite. Therefore, the hydration products increase with the alite content in SRC pastes.
The free lime contents of the cement pastes immersed in 4 % MgSO4 solution up to 9 months are graphically plotted in Figure (2). The results indicate that the free lime of (Cement A) and (Cement B) decreases with time up to 6 months and then increases due to the reaction of Ca(OH)2 with MgSO4 to give gypsum and Mg(OH)2. The increase of free lime contents after 6 months may be ascribed to the decomposition of calcium silicate hydrate by Mg(OH)2 giving Ca(OH)2 and magnesium silicate hydrate. Therefore, the free lime content increases at latter ages. On the other side (Cement C) has lower values of free lime, which decrease up to 9 months. This means that as the belite content increases the librated Mg(OH)2 can not decompose the formed CSH to give Ca(OH)2.
The total sulphate contents of the cement pastes immersed in 4 % MgSO4 solution up to 9 months are given in Figure (3). The total sulphate content increases for all cement pastes up to 9 months. This is mainly due to the migration of the sulphate ions from the aggressive medium (MgSO4 solution) to the cement pastes which react with C3A and Ca(OH)2 fo